Supporting Information - PNAS · Supporting Information Seto et al. 10.1073/pnas.1109243109 SI Text...
Embed Size (px)
Transcript of Supporting Information - PNAS · Supporting Information Seto et al. 10.1073/pnas.1109243109 SI Text...
Supporting InformationSeto et al. 10.1073/pnas.1109243109SI TextSI Materials and Methods. Elemental analysis. Ca2 and Mg2 con-centrations were determined using optical emission spectroscopy(Mg: 285.213 nm, Ca: 317.933 nm) with inductively coupledplasma (ICP) using an Optima 3000 (Perkin Elmer). 15 mg ofground sea urchin spine were dissolved in 2 ml of 30% HCland 2 ml of 65% HNO3 in a Multiwave microwave disintegra-tion device (Anton Paar). Two samples were disintegrated andeach of them was diluted with 100 mL distilled water. The instru-ment was calibrated with standards Mg 1 & 10 ppm andCa 1, 10, 100 ppm.
SEM.The adult sea urchin spines were fractured using tweezers. Afew fractured sea urchin spines were etched in water overnight atroom temperature. The freshly prepared fracture surfaces andthe etched fracture surfaces of the spines were characterizedby SEM (LEO 1550-GEMINI, LEO Electron MicroscopyGroup). Thin sections of thickness 1,000 nm were prepared usingmicrotomy.
TGA. Thermogravimetry analysis measurements were performedwith a Netzsch STA 429 (Netzsch GmbH) in the presence of anitrogen atmosphere. Approximately 49 mg of the ground seaurchin spine were weighed and used for the measurements.The sample was heated at a rate of 5 Cmin until a final tem-perature of 1,000 C.
TEM. Sea urchin spines were embedded in Spurr's resin (TEM)and LR-white (HRTEM) by vacuum infiltration. For TEM ana-lysis sections were cut to a thickness of 50100 nm with an RMCultramicrotome using a diamond knife. Sections were floatedonto either water or ethylene glycol and collected onto 3 mm cop-per mesh grids. TEM/HRTEM analyses were performed using aJEOL JEM 1200 EX (JEOL GmbH) and a JEOL JEM-2100F-UHR (JEOL GmbH), respectively.
WAXS/SAXS/USAXS.All (U)SAXS experiments were performed onsamples embedded in PMMA and cut in a transverse directionwith respect to the main spicule axis using a precision low-speedcircular saw (Accutome 5, Struers Tech A/S, Copenhagen, Den-mark). The outer diameter of the spicule section was in the orderof 1.4 mm. The 500 m thick samples were further reduced toapproximately 100 m by careful polishing with high grade paper(SiC 2400) in order to avoid the presence of microcracks whichwere found to be problematic for (U)SAXS analysis. The acces-sible q-range was 0.0010.3 nm1 corresponding to 206300 nmin real space.
WAXS was performed on a Bruker D8 Advance (Bruker AXSGmbh) using a Gbel mirror and parallel beam geometry at40 kV 40 mA.
The laboratory SAXS machine provided a monochromaticbeam of wavelength CuK 0.154 nm (8.041 keV) was reducedto approximately 100 m in diameter at sample position using acombination of three apertures. Several frames were collected insteps of 100 m across the sample to test possible differencesfrom the core to the outer part of the spicule. This enabled aq-space resolution of 0.132 nm1 to be obtained. This corre-sponds to features in the order of 350 nm in real space.
SAXS analysis.Radial profile of the scattered intensity (arbitraryunits) was measured using a low resolution laboratory instrument.
Two regions, indicated on the graph, follow a law of the type I Pq4 (or, log I logP 4 log q) where P is a constant, which istypical for a dense two-phased system with sharp boundaries. Alinear fit of the logarithmic plot was performed within the bound-aries indicated by the dotted lines. The result of the fit is shown bythe dashed lines; the slopes in the log I vs log q plot were 4.01 and3.98 for region 1 and 2 respectively. Similarly, a slope of 2.06was obtained in the intermediate region. In the schematic, region1 is the calcite nanoparticle (blue), whereas region 2 representsoccluded areas within the nanoparticle (pink).
At the ESRF beamline, an X-ray beam monochromatized to awavelength of 0.0995 nm (12.460 keV) was collimated to ap-proximately 200 m in diameter. Two separate measurementsusing both a pinhole camera and a Bonse-Hart setup were com-bined for very high angular resolution, thus spanning a large partof the ultrasmall angle X-ray scattering (USAXS) regime.
X-ray single crystal structure determination. The vertex of a seaurchin spine was mounted on a glass fiber. Intensity data werecollected at room temperature using a STOE Imaging Plate Dif-fraction System IPDS-2 with graphite monochromatized MoKradiation ( 0.71073 ) at 50 kV and 40 mA (180 frames, 1, 1 min exposure time per frame). The data were cor-rected by a spherical absorption correction using the programX-Area (Stoe, 2004) as well as for Lorentz, polarization and ex-tinction effects. The structure was solved with SHELXS-97 usingdirect methods and refined with SHELXL-97 (S1). All atomswere refined anisotropically. At the beginning, the refinementwas performed only with calcium as the cation. After convergenceof the refinement, magnesium was introduced on the cation sites.The sum of the site occupation factors (sofs) of Ca and Mg wasconstrained to equal the full occupancy of the cation site. Finally,the Ca and Mg site occupation factors were refined free to give asof ratio of 0.96 to 0.04 (Ca to Mg). The unit cell parameters wereestimated with 3,182 reflections. Further details of the crystalstructure investigation may be obtained from Fachinformations-zentrum Karlsruhe, 76344 Eggenstein-Leopoldshafen, Germany[(fax: (+49)7247-808-666; e-mail: [email protected],http://www.fiz-karlsruhe.de/request_for_deposited_data.html]onquoting the deposition number CSD-419785.
SAXS/WAXS analysis. The 2D SAXS patterns were corrected fordetector artifacts, normalized and azimuthally averaged usingthe FIT2D software package (S2) for the SAXS dataset and asoftware package developed at the ID02 beamline (S3) for theUSAXS measurements. The 1D radial profiles were then ana-lyzed using additional software, written in Python language, de-veloped by one of the authors (A. Gourrier) for SAXS/WAXSanalysis.
While the sharp peaks measured with WAXS only yield dimen-sions from the coherently scattering parts of a sample, SAXS pro-vides coherence lengths of volumes where the average electrondensity differs from the bulk, independently of the relative degreeof ordering. The intensity of the SAXS signal therefore directlydepends on the difference in the electron density between the twophases. In order to check for the possibility of measuring a signaloriginating from the ACC fraction in the calcite surrounding, thescattering contrast was calculated. A value of 9.2:1010 cm2was found, based on mass densities of 2.71 gmL for calcite and1.62 gmL for ACC (S4) (neglecting Mg2 and water in theACC), which is sufficient to observe the ACC phase.
Seto et al. www.pnas.org/cgi/doi/10.1073/pnas.1109243109 1 of 11
The analysis of the region of the radial profile at high q (region2 in Fig. 3) was performed by subtracting the contribution at lowq using a law of the form: I P1q4. The resulting curve isshown in Fig. S9 (Top left). This allowed calculating a correlationlength according to a procedure described previously (36)and defined by: T 4JP where P limqq4Iq and J 0 q
Nano-X-ray diffraction (nano-XRD).A transverse section of approxi-mately 50 m was prepared using the protocol described in theSAXS measurements section of the SI. This section was mountedon a translation stage which is, itself, fixed to a rotation stageat beamline ID13 (ESRF). The 2D data were collected using aFrelon detector of 2K 2K pixels with size of 50 50 m2 andprocessed with the softwares Fit2D and PySXIm (custom de-signed Python software) after removal of the parasitic scattering.
A X-ray beam at beamline ID13 (ESRF) was monochroma-tized to an energy of 15.26(5) keV ( 0.8122 ) and focusedin two steps using Be lenses and parabolic X-ray refractive lensesto a focal spot size of 70 nm at FWHM (S6). Sample regions wereidentified using an online optical microscope and the sample-to-detector distance was calibrated using AgBh (S7).
Due to the single-crystalline nature of the sample, two differ-ent measurements were undertaken:
Measurement type 1: Estimation of the degree of rotationaldisorder in a localized volume: Rough rotational scans were ac-quired about the radial direction of the sample () within 5with 0.1 steps in order to locate a diffraction spot of interestin reciprocal space (Fig. S9C). The sum of the 2D patterns withinthis rotational range is shown in Fig. 2A. The sample was thenpositioned to the position MAX of maximum peak intensity(Fig. S9C, Left) and scanned within 1 with finner steps of0.02. The intensity peak profile was calculated by integratingthe intensity within a narrow region of interest around the peak(30 30 pixels). The FWHM in the direction was calculated tobe 0.10 (Fig. S9C, Top right). At the maximum intensity position,the azimuthal profile was calculated (Fig. S9C, Bottom right) with-in the cake region indicated in Fig. S9C, Center. The FWHM wascalculated to be 0.73. Due to the sample thickness, it is assumedthat the number of nanocrystals in the volume probe by the beamis in the order of 500 when the beam is normal to the samplesection. In order enhance the accuracy of the measurement, thismeasurement was repeated with a beam translated laterally bysteps of 5 m over a distance of 60 m. The results remain essen-tially unchanged. Both measures are thus sufficient to fully char-acterize the 3D extent of the peak.
Measurement type 2: In order to obtain a more statistical viewof the regularity in crystalline orientation, a line scan was re-corded along the radial direction of the spicule section, from thecentre to the outermost part, indicated by the red dots in Fig. S9B.This scan was performed at the MAX peak intensity value. Theresults are summarized in Fig. S9D. It can be observed that thepeak position varies within a range of 0.18 (99% of thedata) only over a distance of 600 m. Similarly, the FWHM variesby 0.2 (99% of the data).
-Computer tomography (-CT). A single adult Authoeidaris Eras-sispina sea urchin spine was oriented with UV-cured dental epoxysuch that its longitudinal axis was perpendicular to the incomingX-ray beam. A Skyscan 1072 -CT table-top scanner (Skyscan)was used to scan the dry sample for approximately 5 h (with in-tegration times of 4 s and obtaining 824 images using a cone-beam geometry). Following reconstruction, volume renderingand visualization of the 3D microstructure were performed withAmira 4.0 (Mercury Computer Systems).
Atomic force microscopy. Representative adult sea urchin and cal-cined were embedded in PMMA [poly(methyl methcrylate)].Each sample was sectioned with a 300 m diamond blade usinga low-speed saw (Isomet Low Speed Saw, Buehler Ltd.) perpen-dicular to the longitudinal plane of tranverse plane. The sec-tioned surfaces of each sample were polished with 3 m and 1 mdiamond particles (DP-Spray P, Struers A/S, Ballerup), respec-tively, with an automatic polisher (Logitech PM5, LogitechLtd.) until the average surface roughness was approximately1 m. Surface topology imaging with an atomic force microscopy(Dimension 3100, Veeco Instruments) along the diameter of eachspine was performed on the polished surfaces.
Focused ion beam. Powdered samples were placed onto 400 meshcopper TEM grids (Quantifoil Micro Tools GmbH) coated withcarbon. The TEM grids with samples were placed onto a customTEM grid sample holder and placed into a FESEM (Zeiss Cross-Beam 1540XB, Zeiss SMT GmbH) equipped with a Ga ion30 kV FIB column. Areas of 60 60 m regions (area betweenmesh) were exposed to Ga ion exposure at specific doses. AfterFIB treatment, the sample grids were examined under a TEM.
Details of the NMR analysis. Repetition times of 60 s, 300 s, 600 s,3,600 s and 7,200 s were used for the direct excitation using a 13C90 pulse length of 6 s.
For the 1Hf13Cg cross-polarization (CP) measurements, 12 ktransients were acquired with CP times of 1 ms and 8 ms usingTPPM decoupling. The 1H 90 pulse length was 4 s and repeti-tion times of 2 s were used. The 1H spin lock pulse was rampeddown to 50% during CP to broaden the CP match condition. The13C chemical shifts were referenced using adamantane (CH signalset to 38.5 ppm relative to TMS) as a secondary standard.
Fig. S13A shows two NMR spectra acquired with single pulseexcitation (SP) and at different repetition times of 1 min and120 min (spectra in the middle and at the bottom). Both spectraare plotted and normalized to show that the line shape changesconsiderably with increasing repetition time. The 13CNMR line isbroad for the short repetition time of 1 min, whereas a narrowcomponent appears in addition for the spectrum acquired with120 min relaxation delay (Bottom). Obviously, the spectrum mustconsist of two differently relaxing components. In fact, two timeconstants are obtained for the 13C spin-lattice relaxation behavior(not shown here): (i) one time constant with about 102 min forthe narrow line at 168.55 ppm, and a second time constant ofabout 5 min for the broader line. In addition, 1Hf13Cg cross-po-larization (CP) is effective in this sample. The 1 ms CP spectrumis shown as a top trace in Fig. S13A). This CP line is slightly down-field shifted in comparison with the two other components and ithas about a 30% larger line width compared with the broader ofthe other two lines (cf. Table 1). More importantly, the CP effectis very low such that out of all 13C in the sample, only a minor partis contained in that structure for which we assume is ACC.
The line widths and positions of the fast relaxing broad andextraordinarily long relaxing narrow components were obtainedby subtracting the two spectra (1 min and 120 min repetitiontimes) from each other with proper scaling factors such thateither the narrow or the broad component remain. The resultof the procedure is shown schematically in Fig. S13B for the13C NMR spectrum with 120 min repetition time. These two dif-ferent line shapes show the narrow and broader components se-parated, and these two spectra were then fitted separately using asingle Gaussian for each of these lines to get reliable parametersfor widths and positions. This difference procedure was chosenbecause a simple fit does not yield unique values for positionsand width as the lines overlap strongly. Finally, the 13C MASNMR spectrum was fitted using fixed line positions and widthsfor these two lines and a third, broader component to take intoaccount the CP spectrum. The relative peak areas for the three
Seto et al. www.pnas.org/cgi/doi/10.1073/pnas.1109243109 2 of 11
lines are listed in Table 1; the numbers in the last column give therelative amounts of carbons in these three lines. However, a T1intensity correction factor is required for the narrow line at168.55 ppm because two 13C MAS NMR spectra with relaxationdelays of 60 min and 120 min were added to increase the signal-to-noise ratio (equal number of scans in each experiment). These
delays are on the order of the T1 time of the narrow signal(102 min). Hence, the T1 intensity correction factor amounts to1.84 (for the narrow line only) and is the average of 1.44 11 exp120102 and 2.24 11 exp60102; T1 relaxationtime: 102 min, repetition times in experiments: 120 min and60 min, respectively.
1. Sheldrick GM, Schneider TR (1997) SHELXL: High resolution refinement. Method En-zymol 277:319343.
2. Hammersley AP (1997) ESRF Internal Report. Report No. ESRF97, HA02T; European Syn-chrotron Radiation Facility: Grenoble Cedex, France.
3. Boesecke, P (2007) Reduction of two-dimensional small- and wide angle X-ray scatter-ing data J. Appl Cryst 40:s423s427.
4. Bolze J, et al. (2002) Formation and Growth of Amorphous Colloidal CaCO3 PrecursorParticles as detected by Time-resolved SAXS. Langmuir 18:83648369.
5. Porod G (1952) Die Rntgenkleinwinkelstreuung von dichtgepackten kolloiden Sys-temen. II. Teil. Kolloid Z. 125:5157.
6. Schroer, et al. (2005) 'Hard x-ray nanoprobe based on refractive x-ray lenses. Appl Phys
7. Blanton, et al. (1995) JCPDSInternational Centre for Diffraction Data round robin
study of silver behenate. A possible low-angle X-ray diffraction calibration standard.
Powder Diffr 10:9195.
8. Li X, Xu ZH, Wang R In situ observation of nanograin rotation and deformation in
nacre. (2006) Nano Lett 6:2301.
9. Glatter O, Kratky O (1982) Small-Angle X-ray Scattering (New York, Academic).
Fig. S1. SEM images of the fracture surface of sea urchin spine from other authors in the literature. The yellow circles highlight crystalline-like facets amongthe chonchoidal fracture surfaces.Top image from: Weiner S, Addadi L (1997) J. Mater. Chem., 7, 689-702. http://dx.doi.org/10.1039/A604512J. Reproduced bypermission of The Royal Society of Chemistry. Scale bar=10 m. Bottom image from: Lowenstam HA, Weiner S (1989) On Biomineralization, by permission ofOxford University Press, Inc, www.oup.com. Scale bar=10 m.
Seto et al. www.pnas.org/cgi/doi/10.1073/pnas.1109243109 3 of 11
Fig. S2. Cleavage planes of a single crystal sea urchin spine replica (Upper) and a cleavage plane of geological calcite (Lower). The flat f104g cleavage planesare clearly visible. The yellow circle shows the similar f104g fracture to those observed in Fig. 1A (circles) and Fig. S1.
Fig. S3. FIB effects on the microstructure of sea urchin spine samples (A) TEMmicrograph of a powdered sample from a sea urchin spine without FIB[scale bar 100 nm] (B) Electron diffraction pattern of (A) (C) TEM micrograph of a powdered sample from a sea urchin spine with FIB exposure at 50 A sec cm2 [scale bar 100 nm] (D) Electron diffraction pattern of (C) (E) TEM micrograph of a powdered sample from a sea urchin spine with FIB exposure at500 A sec cm2 [scale bar 200 nm] with areas of microstructural beam damage highlighted in yellow (F) Electron diffraction pattern of (E).
Seto et al. www.pnas.org/cgi/doi/10.1073/pnas.1109243109 4 of 11
Fig. S4. AFM amplitude and phase images of a polished native and calcined (T 450 C) sea urchin spine transverse plane at different magnifications (A)(B.)Granular structures can be observed in the amplitude images of the native spine at various magnifications similar to observations by Wang and coworkers innacre (S8) (C) The corresponding phase image of (B.) highlighting the different mechanical stiffness of the granular structures (D)(E.) Calcination processesalter the granular structures in the spine, seemingly making the material more homogenous (F) The phase image of (E) showing the homogeneity of themicrostructure.
20 40 60 80 100 1200.0
Fig. S5. Wide angle XRD diffractogram of a powdered sea urchin spine.
Seto et al. www.pnas.org/cgi/doi/10.1073/pnas.1109243109 5 of 11
1200 1000 800 600 400-0.2
v2/v4 = 5.4
Fig. S6. FTIR of a powdered sea urchin spine
Fig. S7. Image from single crystal analysis of a sea urchin spine.
Fig. S8. Radial profile of the scattered intensity (arbitrary units) measured using a low resolution laboratory instrument. Two regions, indicated on the graph,follow a law of the type I Pq4 (or, log I logP 4 logq) where P is a constant, which is typical for a dense two-phased systemwith sharp boundaries. In theschematic, region 1 is the calcite nanoparticle (blue), whereas region 2 represents occluded areas within the nanoparticle (pink).
Seto et al. www.pnas.org/cgi/doi/10.1073/pnas.1109243109 6 of 11
Seto et al. www.pnas.org/cgi/doi/10.1073/pnas.1109243109 7 of 11
Fig. S9. (A) Upper left is the azimuthally integrated intensity I vs q where q 4 sin is the length of the scattering vector, 2 being the scattering angleand the wavelength of the radiation. Upper right is the same display in logarithmic units showing the 4 slope at large angles in agreement with a dense 2-phase system (S9). Bottom left, Porod plot Iq4 vs q4 used to calculate P and Bottom right, the Kratky plot Iq2 vs q used to calculate J. The vertical lines shown inthe Bottom left and Upper right plots respectively show the limits chosen for the calculations of P and the logarithmic slope. (B) Optical micrograph of thetransverse sea-urchin spicule thin section in transmission light and measurement scheme: the X-ray nanobeam was normal to the section and the sample wasrotated about the vertical axis within restricted angular range of . [scale bar 100 m] (C) sum of the diffraction patterns within 5 with 0.1 stepsshowing a part of the full single crystal diffraction signal; position of one of the peaks at maximum intensity defined by the rocking curve; azimuthal profile ofthe reflection (D) max position of the peak monitored in (B) over the length of the radial profile; FWHM of the peak
Seto et al. www.pnas.org/cgi/doi/10.1073/pnas.1109243109 8 of 11
Fig. S10 Thermogravimetric analysis on cleaned, powdered sea spines. This demonstrates the temperature regimes where (A) loosely bound and (B) structuralwater leaves the bulk material as well as when (C) ACC transforms to crystalline calcite. (D) In the temperature range >500 C, calcium oxide formation andchemical and structural decomposition of the sample bulk beings to occur.
Fig. S11 SEM zoom image series for the fracture surface of a previously annealed sea urchin spine for 4 h at 450 C.
Seto et al. www.pnas.org/cgi/doi/10.1073/pnas.1109243109 9 of 11
Fig. S12 Schematic model of spine formation occurring in the adult sea urchin spine (A). From a heterogenous state of aggregated ACC nanoparticles (notdrawn for the sake of clarity) and occluded biomolecules (B), a single, random nucleation event occurs leading to a Mg-calcite nanoparticle with occluded ACCdomains in the regions where polymers could not be further expelled via the crystal growth front. The crystal growth front pushes an ACC layer ahead whichbecomes increasingly rich in occluded macromolecules. Further crystallization is inhibited in analogy to impurities in the zone melting process. (Please note thecolor schemethe pink regions are ACCwith such high level of occludedmacromolecules that crystallization is inhibited.) (C). However, inhomogeneities in thesurface layer might still allow for further local crystallization in the form of mineral bridges through the polymer rich ACC layer. After penetrating this layer,further crystallization of a second nanocrystal can take place and proceed as for the first nanoparticle. Repetition of this process leads to a random network ofnanocrystallites in an ACC matrix, which are covered by an ACC layer and are connected via mineral bridges ensuring crystalline continuity (D). The processcontinues until all ACC nanoparticles have crystallized using this mechanism.
173 172 171 170 169 168 167 166 165
(13C) in ppm
SP 60s (N) SP 7200s (N) CP 1ms (N)
172 171 170 169 168 167 166 165
Fig. S13. (A) Comparison of two single pulse (SP) 13C NMR spectra with repetition times of 1 min (dashed line) and 120 min (solid line) to show the presence oftwo differently relaxing line components and of a 1 ms CP spectrum (dash-dot). All spectra are normalized to show line shape variations. (B) Relaxation timeediting of the experimental 13C line shape: a narrow line at 168.55 ppm typical for pure calcite, and a broader component slightly shifted to 168.74 ppm appear.
Seto et al. www.pnas.org/cgi/doi/10.1073/pnas.1109243109 10 of 11
Fig. S14. Powder XRD diffractogram of synthetic ACC nanoparticles at various temperatures. Of particular interest is the (104) peak width broadening withincreasing temperatureswhen using the Debye-Scherrer to quantify the broadening effects, it confirms an increase in polycrystallinity in the sample withincreasing temperatures.
Table S1. Crystal data, details of intensitymeasurements, and structure refinement
Empirical formula Ca0.96 Mg0.04 C O3formula weight 99.46crystal system trigonalspace group (number) R-3c (#167)cell dimensionsa, 4.9721(10)b, 4.9721(10)c, 16.952(4), deg 90, deg 90, deg 120V , 3 362.94(14)T , K 298Z 6dcalcd, gcm3 2.73, cm1 0.2238radiation (, ) MoK (0.71073)2 range, deg 10.6257.94crystal size, mm 0.4 0.3 0.3no. of reflns measd 841no. of unique reflns 98 (Rint 0.0353)no. of variable parameters 14R (for I > 2I) 0.0142R (for all reflections) 0.0145wR (for all reflections) 0.0332goodness of fit, S 1.142
Seto et al. www.pnas.org/cgi/doi/10.1073/pnas.1109243109 11 of 11http://www.pnas.org/cgi/doi/10.1073/pnas.1109243109